Phase Transformation Study of Aluminium Containing Transformation Study of Aluminium Containing...
Embed Size (px)
Transcript of Phase Transformation Study of Aluminium Containing Transformation Study of Aluminium Containing...
Manuscripts submitted by A.R.Kiani-Rashid, ESOMAT, Germany
Phase Transformation Study of Aluminium Containing Ductile irons by Dilatometry
A.R. Kiani-Rashid , D.V. Edmonds** Department of Materials Engineering, University of Sistan & Baluchestan, Zahedan, IRAN,
E-mail, email@example.com ** Department of Materials Engineering, Univ. of Leeds, UK
The temperature for the start of martensite formation (MS) for three Al-alloyed ductile irons containing
0.48%Al, 4.88%Al and 6.16%Al were determined by high-speed dilatatometry. Microscopic observations
also were used to indicate the effects of aluminium addition on the martensite transformation during
quenching. Various heat treatment cycles, with different continuous cooling and isothermal heat
treatments, were used for the experimental irons to indicate the phase transformation in the solid state. The
examination confirmed that an austenite/martensite transformation occurs for irons containing 0.48%Al
and 4.88%Al. The results indicate that martensitic transformation occurs at about 200C for 0.48%Al and
about 190C for 4.88%Al. Whereas there was no evidence of the martensitic transformation for 6.16% Al.
It was further found that for the 4.88%Al experimental alloy used, isothermal transformation at 350 C for
different soaking times gave a typical bainitic microstructure that increased with increasing time of
Keywords: Phase transformation, Dilatometry, Ductile iron, Aluminium, Martensite, Austenite
Higher tensile strength, better resistance to thermal shock, high graphitising tendency, good
scaling resistance at high temperature and good machinability are some of the advantages which
are obtained by adding Al to cast irons and many suggested uses include exhaust manifolds,
turbo-charger housing, disk brake rotors, brake drum, cylinder liners, camshafts and piston rings.
The satisfactory strength of Al-alloyed ductile irons provides the potential of this low-alloy
ductile iron for elevated temperature service . However, Al-alloyed irons have not been used
fully and effectively in order to gain these advantages, because of difficulties encountered during
casting. However, a clean casting can be obtained by correct design of the gating system which
reduces turbulence in the mould and so prevents the inclusion of oxide films into the casting [1-5].
The exact appearance of the as-cast matrix microstructure of nodular cast irons, comprising
ferrite, pearlite, cementite or a combination of these phases, depends upon chemical composition
and cooling rate. A bullseye structure, which is spheroidal graphite surrounded by ferrite, is the
most probable structure in unalloyed ductile irons. It is believed that the ferrite halo around the
spheroid is formed before the eutectoid transformation. The volume fraction of ferrite increases
as the cooling rate decreases, and fully ferritic structure is possible in heavy section casting .
Further heat treatment may cause more variety from formation of austenitic phase transformation
products such as bainite, martensite or high-carbon retained austenite, which then confer different
physical and mechanical properties on the iron .
It is apparent that the matrix in cast irons is virtually identical to that in steel. As for steel, the
addition of alloying elements can modify the microstructure, and hence the physical and
mechanical properties. As an example, the addition of copper refines the pearlite and promotes a
stronger and harder pearlite. The hardness of ferrite in the pearlite also can show an increase, due
to solid solution hardening. Cu is a graphitising element and accompanied by Si suppresses the
formation of hard carbides. The hardness continues to increase with the formation of pearlitic
matrix as Cu increases and a substantial increase in tensile strength and wear resistance and
excellent machinability also can be achieved. However, the low solubility of copper limits its
application but it can be added with other elements such as nickel [6, 7].
Angus  explained that for a 2 per cent addition of aluminium the pearlite formation
temperature increases about 16 and 96 for 6.2%Al addition. Stefanescu and Martinez 
showed that increasing the aluminium content in the Fe-C-Al system can decrease the level of
intercellular carbides. It has also been illustrated that as the amount of aluminium in
compacted/vermicular graphite cast irons in the Fe-C-Al system was increased, the pearlite
content in the matrix also increased. It has also been reported that the microhardness of pearlite
and ferrite increased with higher Al content, due to solid solution strengthening and a finer
High-speed dilatometry results showed that the austenite reaction is related to the Al content and
that there is no -loop at high Al concentrations; the austenitic reaction and therefore bainite
reaction were not achieved for an iron containing 6.16%Al.
2. Experimental Procedures
The melts were cast with a pouring temperature of approximately 1350C by both green sand
moulding and gravity die casting. Standard 12.5 mm and 25 mm Y-block sand moulds and
permanent moulds were used and a bottom gating introduced the metal smoothly into the mould
cavity to ensure a sound casting.
The experimental ductile irons with a range of composition were produced in a Morgan gas -
fired furnace ( with 25 kg capacity lift - out crucible ) and a high - frequency melting plant of 20
kg capacity (with a tilting crucible). After melting, the iron was superheated at 1550C and small
pieces of solid aluminium added by plunging into the bottom of the liquid metal. Enough time
was given to dissolve the aluminium completely in the molten metal. Following aluminium
treatment, FeSiMg(5%Mg) alloy was plunged into the liquid iron and ejection of molten metal
during solution of magnesium prevented by use of special enclosed reaction vessels. Finally,
post-inoculation of ferro-silicon containing 75%Si was carried out in the crucible.
2.2. Chemical composition
Quantitative measurements of the carbon content in the experimental irons were made using
equipment at Swinden Technology Centre of Corus Group PLC (formerly British Steel Ltd.).
Analyses were performed by an infrared absorption method after combustion in an induction
furnace and oxidation to CO2. In order to analyse for aluminum in high-Al content ductile irons,
an atomic absorption spectrophotometry (AAS) method was used by Hi-Search Technology
(HIST) of Birmingham University.
2.3. Sample preparation
Specimens 60x11x11mm for further experimental work were machined using an abrasive wheel
cut-off machine type Cutmaster and a band saw type Qualters & Smith G10. The specimens were
prepared from the bottom section of the experimental keel blocks (Y-blocks) in order to avoid
porosity and segregation effects in the ingots. A Struers Discotom-2 cutting machine was used
for all optical and SEM samples. The specimens were then mounted in bakelite and ground to
1200 grit wet silicon carbide paper followed by polishing to 1m with diamond paste. Phase
identification was achieved after etching in 2% nital. The same techniques were used to prepare
the specimens for hardness measurement.
2.4. Hardness measurements
After impact testing and examination samples with dimensions 20x10x10mm were cut from the
Charpy specimens. Hardness measurements were made on these using a Vickers Engineering
Group Vickers hardness machine at a load of 50 Kg on polished samples. A minimum of five
measurements was made for each sample.
2.5. Microstructural examination
Optical microscopy and SEM were used to examine and delineate any variations in the
microstructure e.g. the shape, size and distribution of nodular graphite, the size and distribution
of bainitic packets and retained austenite, with changes in composition and heat treatment. Nikon
and Reichert-Jung optical microscopes were used for optical metallography. The Nikon D.I.C
(different interference contrast) microscope makes use of polarised light, incorporating polariser,
analyser and compensating plate as in a normal polarised light microscope. To change the colours
of the phases, the polarised dial is rotated until suitable contrast/colour was achieved. For
scanning electron microscopy, a Cambridge Series 3 SEM fitted with a Link 860 series 1 EDX
system and a Cambridge Series 4 SEM were used. For the characterisation of microstructure a
working distance between 20-24 mm was chosen, and an accelerating voltage of 20kv and spot
size between 4 - 6 nm.
Dilatometric experiments were carried out using a Theta Industries high-speed vacuum
dilatometer (Dilatronic III) with rapid gas quenching. Cooling to the target temperatures was
achieved by an automatically controlled high pressure helium jet. The tests were performed on 10
mm by 3 mm diameter tubular specimens with a 1.5 mm diameter bore in the centre to enable fast
quenching. 0.15 mm thermocouple wires were spot welded to the specimens to measure variation
of temperature during the heat treatm